TIG Welding pdf
Embed Size (px)
Transcript of TIG Welding pdf
TIG WeldingKyle Westmoreland Brad Watson
OverviewTIG=Tungsten Inert Gas Welding Uses a tungsten electrode to produce an electric arc. The weld is shielded by a gas typically argon and a welding rod is added to produce the weld Uses TIG welding can be used to weld Magnesium, Aluminum, Steel, Stainless Steel, Brass alloys, Silver, Cast Iron and Copper Can weld very thin sections and metals that can not be easily welded with other types of welding.
Safety Concerns Always be sure to wear flame resistant clothing like cotton when welding. Synthetic materials burn easily and can melt to your skin. Before Welding be sure area is properly ventilated. Use adjustable exhaust fan when welding in shop. Always wear welding gloves and a welding helmet with a lens shade of 10 or 11. Caution: Welding produces high temperatures even after welding is completed Ensure the piece you are welding is safe to weld (ie: a container containing flammable liquid).
Welding AreaHelmets Gas Regulator Exhaust Vent Filler Rods
TIG Welder Electrodes and Gloves
Getting Started Choose the correct electrode and filler rod based on the type of material and thickness of weld (see Aluminum TIG Specifications) Prep surface by removing any corrosion or oil with a wire brush to ensure a clean strong weld. Ensure others around you know you are welding and there is no potentially flammable materials.
Setting up the Machine Steel: Use DC straight polarity and an electrode with a red end (2% Thoriated). When welding steel with DC straight polarity make sure the tip is ground to a conical point (see Preparing Steel Electrode). Aluminum: Use AC current and an electrode with a green end (100% Tungsten) Ensure that the tip is round properly (see Preparing Aluminum Electrode). Other Material: Consult welding reference or experienced welder. *Amperage varies depending on material thickness and type of weld. Aluminum
Aluminum TIG SpecificationsStock Joint Thickness Type 1/16 Butt Lap Corner Fillet 1/8 Butt Lap Corner Fillet 3/16 Butt Lap Corner Fillet 1/4 Butt Lap Corner Fillet Amperes AC Current Horizontal Flat & Vertical Overhead 60-80 60-80 60-80 70-90 55-75 60-80 60-80 60-80 60-80 70-90 70-90 70-90 125-145 115-135 120-140 140-160 125-145 130-160 125-145 115-135 130-150 140-160 115-135 140-160 190-220 190-220 180-210 210-240 190-220 180-210 190-220 180-240 180-210 210-240 190-220 180-210 260-300 220-260 210-250 290-340 220-260 210-250 280-320 220-260 210-250 280-320 220-260 210-250 Argon Flow(20psi) Electrode (in.) 1/16 1/16 1/16 1/16 3/32 3/32 3/32 3/32 1/8 1/8 1/8 1/8 3/16 3/16 3/16 3/16 lpm 7 7 7 7 8 8 8 8 10 10 10 10 12 12 12 12 cfh 15 15 15 15 17 17 17 17 21 21 21 21 25 25 25 25 Filler Rod(in) 1/16 1/16 1/16 1/16 1/8 1/8 1/8 1/8 5/32 5/32 5/32 5/32 3/16 3/16 3/16 3/16
*Miller,R.T. Welding Skills 2nd Edition. 1997 American Technical Publishers Inc. Homewood, Illinois 60430
Note: When welding thicker aluminum with shop welder(>.25 in) try to preheat material with oxy-acetylene torch.
Adjusting Torch Insert electrode by unscrewing the end of the torch and then sliding electrode into the collet. For general use the electrode should extend 1/8 to 3/16 of an inch beyond the cup to ensure the shielding gas shields the weld.
Preparing Steel Electrode Make sure tip is free for build up and ground to fine point Using machine sharpening grinder to grind to a pointCorrect Tip Incorrect Tip
2.5 x Diameter
Preparing Aluminum Electrode Aluminum tip created using a piece of copper to generate an arc. Set amperage to max setting. Hold Electrode 1/8 in from copper and press peddle. Heat generated causes tip to melt in to smooth ball.Correct Tip Incorrect Tip
Hold torch approximately 75-80 degrees from horizontal and the filler rod 15-20 degrees from horizontal.
Welding Technique Hold the tip of the electrode about 1/8 away from piece and press the pedal down until an arc is created between the electrode and work piece. Keep peddle depressed until puddle is created. Ensure the tip of the electrode does not touch the molten weld puddle. This cause electrodes to become contaminated with weld material.
Welding TechniqueAfter puddle is created use a circular motion or repeated crescent motion to move puddle while adding filler rod. When welding thinner materials a heat sink, consisting of a metal block, can be used to dissipate excess heat. Place this heat sink underneath material when welding.
Additional References Mentors for 2005-2006: Phil Arpke Mike Harper
Books Miller,R.T. Welding Skills 2nd Edition. 1997 American Technical Publishers Inc. Homewood, Illinois 60430 Welding Skills 2nd Edition Author: R.T. Miller Publisher: American Technical Publishers Inc.
U of I Course Agricultural Systems Management 107 (ASM 107)
Thanks to:Phil Arpke Adrian Gomez Mike Harper Russ Porter